A Study on Mechanical and Microstructural Characteristics of Concrete Using Recycled Aggregate

The objective of this paper is to provide a comprehensive study about the performance of concrete using mixed coarse recycled aggregate (MCRA) as an alternative for natural aggregate (NA) at replacement levels of 0, 30, 60, and 100%, which can greatly reduce the environmental pollution by incorporating the construction and demolition wastes in the reproduction of concrete. The focus of this study was to use the raw MCRA that was directly obtained from a recycling plant and not further processed. Initially, MCRA was studied to ascertain if its property meets the recommended Indian standards for natural aggregates. Using the slump test, the workability of freshly prepared concrete with a characteristic strength of 30 MPa was assessed. Additionally, the mechanical performance of concrete was assessed on the specimens prepared in the different forms: cubes, cylinders, and beams. Moreover, Scanning Electron Microscopy (SEM) with EDAX, XRD, and FTIR were used to study the microstructural behavior of selected optimum and control mixes at 7 and 28 days of curing. The studies revealed that a higher MCRA content improved the workability of concrete and 30% replacement of MCRA improved the compressive strength by 11.01, 6.98, 6.19, and 14.24% at 7, 28, 56, and 90 days respectively. At the same time, the 30% replacement of the MCRA mix showed an improved split tensile and flexural strength by 2.92 and 6.26%, respectively. The microstructural analysis showed that the optimum mixture had a more condensed microstructure. Therefore, 30% replacement of MCRA can be incorporated in the characteristic strength of concrete of 30 MPa. In particular, MCRA incorporation had a positive influence similar to conventional concrete on the physical, mechanical, and microstructural properties, which can increase the utilization of all kinds of directly obtained construction and demolition wastes to increase the circular economy in the construction sector.


Introduction
Concrete is a human-made substance that is the most widely used material on the planet. At the same time, unfortunately, it represents a source of concern when it comes to environmental degradation. It is of maximum importance to investigate the materials used to manufacture concrete, as well as their broader environmental impact. It is expected that global annual construction waste could reach 2.2 billion tons by 2025 as reported by transparency market research. Based on the report of the building materials and technology promotion council [1], India produces approximately 150 million tons of Construction and Demolition Waste (C&DW) every year. As the rate of demolition of old structures has increased, enormous amounts of C&DW debris have been generated [2,3]. In most

Experimental Program
The experimental study incorporated concrete with a varied percentage of recycled aggregates at 0, 30, 60, and 100 to determine the effect of recycled aggregate concrete at low, moderate, and high volumes. In this research, the mechanical properties of mixed recycled aggregate concrete such as compressive, flexure, and split tensile strength were investigated. Furthermore, nondestructive parameters of selected concrete series were evaluated in terms of the ultrasonic pulse velocity and rebound hammer. The morphology and cement hydration products of the optimum and control mix were studied using Scanning Electron Microscopy with Energy-Dispersive X-ray Spectroscopy (SEM-EDAX), X-ray Diffraction (XRD), and Fourier Transform Infrared Radiation (FT-IR).

Materials
In this current research, mixed coarse recycled aggregate was used as an alternative to conventional aggregate, which can increase the incorporation of all kinds of construction and demolition waste in concrete production. The natural aggregates utilized locally from Chennai, India and mixed recycled aggregates were sourced from the C&DW Recycling Plant at Jeedimetla in Telangana, India. The manufactured sand with a size less than 4.75 mm that belongs to Zone I as per IS383:2016 was used in this research. During the production of the reprocessed aggregates, the unsettled substances were discarded first from C&DWs and, thereafter, the construction waste was crushed by a jaw crusher and separated according to their sizes. The recycled aggregates involved in this study contained all forms of construction and demolition wastes except steel and floating materials. The coarse mixed recycled aggregates of 20 mm and 12 mm were mixed at a percentage of 60% and 40%, respectively, to enhance the properties of recycled aggregate concrete with better packing. Ordinary portland cement (53 grade) manufactured by Zuari, meeting IS 12269:2013 requirements, along with tap water was used for the experimental process. The superplasticizer (SP) with trading name AURAMIX 200 was used with a solid content of 30-35% having a specific gravity 1.08, which has a 20% water reduction rate. The amount of SP was found on the basis of workability requirements.
The coarse recycled material used in this study is shown in Figure 1. The typical composition of the recycled aggregate sample that was collected from the C&DW recycling plant at Jeedimetla, India was 73.8% fully reclaimed aggregate, 16% aggregate with partially adhered mortar, 4.45% tiles, 1.07% bricks, 1.63% black stones, 2.47% granite, 1.08% mosaic, and 1.97% others. and cement hydration products of the optimum and control mix were studied using Scanning Electron Microscopy with Energy-Dispersive X-ray Spectroscopy (SEM-EDAX), X-Ray Diffraction (XRD), and Fourier Transform Infrared Radiation (FT-IR).

Materials
In this current research, mixed coarse recycled aggregate was used as an alternative to conventional aggregate, which can increase the incorporation of all kinds of construction and demolition waste in concrete production. The natural aggregates utilized locally from Chennai, India and mixed recycled aggregates were sourced from the C&DW Recycling Plant at Jeedimetla in Telangana, India. The manufactured sand with a size less than 4.75 mm that belongs to Zone I as per IS383:2016 was used in this research. During the production of the reprocessed aggregates, the unsettled substances were discarded first from C&DWs and, thereafter, the construction waste was crushed by a jaw crusher and separated according to their sizes. The recycled aggregates involved in this study contained all forms of construction and demolition wastes except steel and floating materials. The coarse mixed recycled aggregates of 20 mm and 12 mm were mixed at a percentage of 60% and 40%, respectively, to enhance the properties of recycled aggregate concrete with better packing. Ordinary portland cement (53 grade) manufactured by Zuari, meeting IS 12269:2013 requirements, along with tap water was used for the experimental process. The superplasticizer (SP) with trading name AURAMIX 200 was used with a solid content of 30-35% having a specific gravity 1.08, which has a 20% water reduction rate. The amount of SP was found on the basis of workability requirements.
The coarse recycled material used in this study is shown in Figure 1. The typical composition of the recycled aggregate sample that was collected from the C&DW recycling plant at Jeedimetla, India was 73.8% fully reclaimed aggregate, 16% aggregate with partially adhered mortar, 4.45% tiles, 1.07% bricks, 1.63% black stones, 2.47% granite, 1.08% mosaic, and 1.97% others.

Physical Properties Studied
The physical properties of the aggregates obtained from the construction and demolition recycling plant at Jeedimetla were studied and the results are shown in Table 1. From the results, it can be observed that the mixed coarse recycled aggregates (MCRA) exhibited an almost similar nature compared to natural aggregates (NA). However, the water absorption of the MCRA was much higher than that of the NA. The 24 h water

Physical Properties Studied
The physical properties of the aggregates obtained from the construction and demolition recycling plant at Jeedimetla were studied and the results are shown in Table 1. From the results, it can be observed that the mixed coarse recycled aggregates (MCRA) exhibited an almost similar nature compared to natural aggregates (NA). However, the water absorption of the MCRA was much higher than that of the NA. The 24 h water absorptions of MCRA of sizes 20 mm and 12 mm were 2.3% and 1.95%, which were higher than those of NA. Table 1 shows the water absorption of recycled aggregates in the present study, which is the same as those of the studies accomplished by various authors described in Table 2. The bulk density of MCRA was reduced at a percentage of 10.58% and 18.38% for 20 mm and 10 mm, respectively, compared with NA. Recycled aggregates showed a density reduction and a notably higher water absorption than NA. In addition, the aggregate crushing and impact value was almost twice the value of NA. Even though the physical properties differed when compared with natural aggregate, the strength properties were not affected significantly for recycled aggregate concrete [32]. This was because of the bond strength as the roughness of the aggregate increases [33]. However, the specific gravity of those recycled aggregates was similar to those of natural aggregates varying from 2.1 to 3.2 and satisfied the permissible limits IS 383:2016.

Granulometric Distribution of Aggregates (NA and MCRA)
The particle size distributions of aggregates were determined using a sieve analysis test as per IS 383:2016. Figure 2 shows the various size ranges of all aggregates (both fine and coarse aggregates) for the 100% natural and mixed coarse recycled aggregate (MCRA) concrete mix compared with the upper and lower limits specified by IS 383:2016. The cumulative passing of all aggregates (both coarse and fine) for 100% natural and MCRA in the corresponding sieve size of 40, 20, 4.75, 0.6, and 0.15 mm was 100, 98.09, 40, 17.56, and 4.72% and 100, 88. 45, 11.34, 14.80, and 1.52%, respectively. For the 100% MCRA curve, the gradation value deviated from the upper and lower limits in the sieve size of 4.75 mm at 11.35%. In addition, the deviation in the sieve size of 20 mm was 6.9%, which almost coincided with the lower limits. Despite the fact that the gradation differed from the control and did not meet the limits of grading requirements, the gradation was similar, indicating consistent RA generation. In addition, we chose to use the RA to make concrete without changing the gradations, which was supplied from the C&DW recycling plant. The choice was made to save expenditure and to make use of available gradations to achieve an acceptable particle distribution.
the corresponding sieve size of 40, 20, 4.75, 0.6, and 0.15 mm was 100, 98.09, 40, 17.56, and 4.72% and 100, 88.45, 11.34, 14.80, and 1.52%, respectively. For the 100% MCRA curve, the gradation value deviated from the upper and lower limits in the sieve size of 4.75 mm at 11.35%. In addition, the deviation in the sieve size of 20 mm was 6.9%, which almost coincided with the lower limits. Despite the fact that the gradation differed from the control and did not meet the limits of grading requirements, the gradation was similar, indicating consistent RA generation. In addition, we chose to use the RA to make concrete without changing the gradations, which was supplied from the C&DW recycling plant. The choice was made to save expenditure and to make use of available gradations to achieve an acceptable particle distribution.

Mix Design
Four mixes were composed to explain the concrete in the fresh state, the hardened properties, and the microstructural behavior of concrete. The specimens were prepared in the different combinations: control mix with 100% NA; concrete with 30% MCRA (M1); concrete with 60% MCRA (M2); concrete with 100% MCRA (M3). The proportion of the mixes was designed using IS 10262:2019 shown in Table 3. All the mixes were designed to meet severe environmental conditions with an amount of binder of 380 kg/m 3 and a water-cement ratio of 0.42 as per IS 456:2000. The mixes studied were prepared using a 45 L capacity laboratory vertical shaft mixer. All the dry ingredients were loaded one by one and dry-mixed for a duration of 120 s, and then water was added while the mixer was running; simultaneously, the superplasticizers were added to improve the workability. The total mixing time was 240 s, which satisfied the minimum requirement as per IS 456:2000. Finally, the samples were produced and cured by following IS 456:2000.

Mix Design
Four mixes were composed to explain the concrete in the fresh state, the hardened properties, and the microstructural behavior of concrete. The specimens were prepared in the different combinations: control mix with 100% NA; concrete with 30% MCRA (M1); concrete with 60% MCRA (M2); concrete with 100% MCRA (M3). The proportion of the mixes was designed using IS 10262:2019 shown in Table 3. All the mixes were designed to meet severe environmental conditions with an amount of binder of 380 kg/m 3 and a water-cement ratio of 0.42 as per IS 456:2000. The mixes studied were prepared using a 45 L capacity laboratory vertical shaft mixer. All the dry ingredients were loaded one by one and dry-mixed for a duration of 120 s, and then water was added while the mixer was running; simultaneously, the superplasticizers were added to improve the workability. The total mixing time was 240 s, which satisfied the minimum requirement as per IS 456:2000. Finally, the samples were produced and cured by following IS 456:2000.

Results and Discussion
Fresh concrete properties, namely slump and density, were determined as specified in IS 456:2000. All the mixes were planned to have a retention slump value of one hour by fixing the dosage of superplasticizer (SP) ARAMIX 200 at 0.4% in the amount of binder. The variation in slump is shown in Figure 3. The slump loss range of all the mixes at different time intervals 0, 15, 30, 45, and 60 min is shown in Figure 4. In the graph of Figure 4, the mixes with recycled aggregates show higher slump values than the control mix due to more water absorption, which, in turn, increases the free water available for hydration [38]. All the mixes show an initial collapse with 0.4% of SP and, after one hour, all the mixes have a slump value around 75 ± 20 mm due to the absorption nature of recycled aggregates. The fresh density of all the mixes is nearer to that of conventional concrete, as shown in Table 4. Even the mix with 100% RA has a fresh density of 98% compared to that of conventional concrete. From these obtained results, it is worth noting that the fresh density is within the range of 2430-2300 kg/m 3 for concrete that has different replacements of RA. This finding denotes that the tiles, mosaic, granite, and other components present in RA do not compromise the density of freshly prepared concrete. A similar study reported that the compressive strength of 25 MPa concrete showed a fresh density of 2416 and 2331.01 kg/m 3 for ordinary concrete and 50% replacement of mixed recycled aggregate concrete (MRAC), respectively. The previous studies [16] found that the bulk density for the fresh concretes was 2.45 Mg/m 3 for conventional and 2.28 Mg/m 3 for 100% replacement of MRAC. Thus, it was found that the fresh concrete replaced with recycled aggregate has suitable properties for application of concrete.
Fresh concrete properties, namely slump and density, were determined as specified in IS 456:2000. All the mixes were planned to have a retention slump value of one hour by fixing the dosage of superplasticizer (SP) ARAMIX 200 at 0.4% in the amount of binder. The variation in slump is shown in Figure 3. The slump loss range of all the mixes at different time intervals 0, 15, 30, 45, and 60 min is shown in Figure 4. In the graph of Figure  4, the mixes with recycled aggregates show higher slump values than the control mix due to more water absorption, which, in turn, increases the free water available for hydration [38]. All the mixes show an initial collapse with 0.4% of SP and, after one hour, all the mixes have a slump value around 75 ± 20 mm due to the absorption nature of recycled aggregates. The fresh density of all the mixes is nearer to that of conventional concrete, as shown in Table 4. Even the mix with 100% RA has a fresh density of 98% compared to that of conventional concrete. From these obtained results, it is worth noting that the fresh density is within the range of 2430-2300 kg/m 3 for concrete that has different replacements of RA. This finding denotes that the tiles, mosaic, granite, and other components present in RA do not compromise the density of freshly prepared concrete. A similar study reported that the compressive strength of 25 MPa concrete showed a fresh density of 2416 and 2331.01 kg/m 3 for ordinary concrete and 50% replacement of mixed recycled aggregate concrete (MRAC), respectively. The previous studies [16] found that the bulk density for the fresh concretes was 2.45 Mg/m 3 for conventional and 2.28 Mg/m 3 for 100% replacement of MRAC. Thus, it was found that the fresh concrete replaced with recycled aggregate has suitable properties for application of concrete.

Initial Slump
After 30 min After one hour       The hardened density values shown in Table 5 vary from 2532.74 to 2461.04 kg/m 3 for the mix having NA and MRAC. In comparison with the control mix, the dry density of 30, 60, and 100% replacements of recycled aggregates decreases by 2.83, 2.78, and 1.6% respectively. This decrease in density is closer to the previous study by [17], which reported that the dry density of hardened concrete was 2416.37 and 2331.01 kg/m 3 for the control and 50% replaced MRAC, respectively. This indicates that there was a 3.5% reduction in apparent dry density of MRAC while comparing with conventional concrete. The results of the current study show that the decrease in dry density of MRAC is less than the results obtained in previous studies. Figure 5 demonstrates how the compressive strength of each recycled aggregate concrete mix increases over time in a manner comparable to the behavior of reference concrete. As shown in Figure 5, the compressive strength of recycled aggregate decreases beyond 30% replacement of MCRA, which can be attributed to the alteration in the watercement ratio of the mix due to the higher water absorption of recycled aggregates during concreting. From Table 5, it can be observed that at 7, 28, 56, and 90 days, the strength of group M1 increases by 11.01, 6.98, 6.19, and 14.23% compared with the control mix. The relative compressive strength of all mix groups after seven days is in the range of 64.47-76.6% as that obtained after 28 days. At the 28th day, all the mixes satisfy the design strength of 30 MPa. The resulting design strength of MRAC was also achieved by an earlier study, which stated that even when the natural aggregate replacement percentage exceeded 80%, the mechanical performance of the recycled concrete generated with coarse recycled aggregates was comparable to that of regular concrete [39]. Further, at the 56th day, the strength increases at a percentage of 11.95, 19.01, 13.75, and 12.78% for M1, M2, M3, and the control mix, respectively, when compared to the 28th day's compressive strength of each mix. Similarly, the 90th day strength increases at a percentage of 12.94, 10.7, 6.59, and 4.99% for M1, M2, M3, and the control mix, respectively, when compared to the 56th day's compressive strength of each mix. However, compared with the control mix, it is observed that the compressive strength gradually decreases with increasing replacement percentage of MCRA in the concrete mixes. The reduced compressive strength obtained in the MRAC is because of the fact that recycled aggregate has different heterogenous components in the aggregate portion. As a result, the strength of concrete made with recycled aggregate is generally decreased by the interaction between the old mortar and fresh cement paste. Therefore, it is necessary to address the complex interaction behavior of recycled aggregate concrete. However, all of the mixes meet the design strength requirements on all curing days. Similar observations have been reported in previous studies by [17] who reported that after 28 days, the average strength was more than the 25 MPa design strength. As a result, these new recycled concretes might be utilized as structural concrete. Previous studies have demonstrated similar patterns in compressive strength gains across all age groups, regardless of the proportion of natural coarse aggregate replaced by recycled concrete aggregate. The same trend can be observed with the use of mixed recycled aggregate in this current study. Based on these observations, we conclude that the MCRA can be effectively used in structural applications. structural concrete. Previous studies have demonstrated similar patterns in compressive strength gains across all age groups, regardless of the proportion of natural coarse aggregate replaced by recycled concrete aggregate. The same trend can be observed with the use of mixed recycled aggregate in this current study. Based on these observations, we conclude that the MCRA can be effectively used in structural applications.

Split Tensile and Flexural Strength
The bending and split tensile strength tests were carried out without applying any shock, and the load was gradually increased at a nominal rate between 1.2 and 2.4 N/mm 2 /min. The differences in strength compared to the control mix are shown in Table  6 along with the split tensile and flexure strengths of concrete tested after 28 days. From the results tabulated, it is evident that the higher amount of recycled aggregate in concrete

Split Tensile and Flexural Strength
The bending and split tensile strength tests were carried out without applying any shock, and the load was gradually increased at a nominal rate between 1.2 and 2.4 N/mm 2 /min. The differences in strength compared to the control mix are shown in Table 6 along with the split tensile and flexure strengths of concrete tested after 28 days. From the results tabulated, it is evident that the higher amount of recycled aggregate in concrete results in a decrease in the strength of the interfacial transmission zone (ITZ). The tensile strength of MRAC is often lower than that of natural aggregate concrete. The extent of the difference depends on a number of variables, including the percentage of recycled aggregate replacement, waterreducing admixtures, and the impact of crushing and mixing processes [40]. Furthermore, from the obtained results, the concrete mix having 30% MCRA shows slightly better performance than the control mix both in flexural and split tensile strength. Similarly, in a previous study, it was found that the tensile strength of concrete produced with recycled coarse aggregate was nearly identical to that of concrete prepared with natural coarse aggregate [41]. In this study, for the concrete having coarse recycled aggregate with 100% replacement, the splitting tensile strength is reduced to 19%. Similar findings were reported with a 18% reduction in splitting tensile strength [42]. This reduction in tensile and split tensile strength of concrete is because of its various components, size, type, and quality. Moreover, the splitting tensile and flexure strength tests on specimens with recycled aggregate shows that the concrete frequently fails through the paste around the recycled aggregate.

Nondestructive Testing
In the present study, nondestructive testing of concrete was assessed as per IS 516 (part 5): 2018. Figure 6 shows the typical arrangement of the test setup for the ultrasonic pulse velocity (UPV) and rebound hammer tests. As shown in Figure 6, two transducers were placed on either side of the concrete specimen in order to assess the homogeneity of concrete specimens. The ultrasonic waves were allowed to pass between the two ends of the transducer to measure the UPV value in terms of m/s. As the side of the cube was 150 mm, the natural frequency of the transducer used here was 150 kHz as per the IS standards. In Table 7, it is seen that at 30% MCRA, the UPV is found to be 4495 m/s, and it slightly increases to 4655 m/s with concrete with 100% NA, i.e., control mix. Similar findings from an earlier study indicated that the reduction in pulse velocity caused by 50% replacement of RCAs in the mix was quite low, i.e., a small drop of up to 6% [43]. The very small decrease in UPV of MRAC at 30% replacement in the current study shows that the recycled aggregate replacement does not alter the phases of calcium silicate hydrate (CSH) in the pores by pozzolanic reaction. The blending of 20 mm and 12.5 mm at 60 and 40% coarse aggregates contributes to the increase in packing density of the cube with minimum voids, leading to better performance.    Figure 6 shows the Schmidt rebound hammer test to measure the surface hardne of the concrete specimens. Table 7 shows the Schmidt rebound hammer value of the sp imen made with 30% replacement of MCRA and 100% natural aggregate. The 28-day   Figure 6 shows the Schmidt rebound hammer test to measure the surface hardness of the concrete specimens. Table 7 shows the Schmidt rebound hammer value of the specimen made with 30% replacement of MCRA and 100% natural aggregate. The 28-day rebound numbers of concrete with 30% incorporation of MCRA and the control mix are obtained as 32 and 36, respectively. The results of the current study are found to be higher than those of an earlier study that reported the 28-day rebound hammer value of concrete mix with 50% incorporation of RCA and control mix to be 26.4 and 23.9, respectively [44]. The lesser difference between the optimum and control mixes in the current study is due to the porous nature of MCRA that results in penetration of the cement paste into it than ordinary concretes.

Scanning Electron Microscopy with Energy-Dispersive Spectroscopy
The morphological characteristics of concrete mixtures were determined on the powder sample of a broken cube for both 7 and 28 days of curing. The TESCAN VEGA3 instrument manufactured from Brno, Czech Republic is used for scanning electron microscopy testing. All the absorbed water in the specimen was removed by hydration stoppage using the oven-drying method at 100 • C for a duration of 10 min. From Figure 7A, at 30% replacement of recycled aggregate concrete, the SEM observation shows that a dense ITZ is present in the layer between the recycled aggregate and the cement matrix. A strong layer of bond between the new cement paste and the aggregate is formed due to the rough surface and high porosity of MCRA, allowing water and cement paste to permeate the aggregate structure. The increase in surface tension results in a stronger bond between recycled coarse aggregate and cement matrix [45]. The increase in adhesion between cement paste and recycled coarse aggregate is due to the formation of hydration product deposits such as calcium silicate hydrate, portlandite, and calcite around the aggregates at such early times as 7 days, which is clearly seen at 30% replacement of MRAC. This is evident from Figure 7A where we see the presence of the large number of these small hydrated crystallites. Due to the creation of massive clusters of hydrated crystals, the voids and pores are filled completely. From Figure 7, we can observe that there is only limited ettringite formation, which is generally responsible for cracks in hardened concrete due to its expansion nature during the hydration process. As the hydration time increases up to 28 days, concrete mix densifies substantially. When compared with the control mix, there is no significant difference at 30% replacement of MCRA. An earlier, similar observation was that there was a stronger and denser new interfacial transition zone with fully replaced coarse recycled aggregates and powdered fine recycled aggregate [46].
The interfacial zone ( Figure 7B), which mainly consists of a large densified layer of hydrates, is similar to that observed by [46]. Beyond 30% replacement of MCRA, the amount and distribution of CSH is insufficient. Thus, the increased replacement of the MCRA results in a large amount of porosity and reduced strength of concrete, which can lower the durability properties that can be seen in Mix 3 at 28 days in Figure 7F. CSH gel decalcifies into silica gel, therefore deteriorating the performance of concrete, which can be seen in Figure 7D at 28 days. The increasing amount of silica gel may produce cracks and loss of durability and mechanical strength in concrete structures. In the case of 100% replacement, the SEM images show more nonhydrated particles due to the incomplete reaction caused by the smaller surface area of the mixture, resulting in a less compact microstructure and strength. Therefore, the increased percentage of recycled content results in inferior properties when compared to the natural concrete.
The energy-dispersive X-ray spectroscopy shows the high content of major peaks of Ca, Si, and O, which indicates the presence of calcium silicate hydrates (CSH) in hardened concrete. The high calcium content shown in Figure 8C indicates the presence of a monolithic amorphous CSH similar to the results reported by [47]. The Ca:Si ratio of the optimum and control mix were calculated from the values shown in Figure 8. At 7 days of curing, the Ca:Si ratio is 0.96 and 0.83 for the optimum and control mix, respectively. After a curing time of 28 days, the results indicate that the Ca:Si ratio of the optimum mix is 2.33 when the control mix results in 1.61. Though the atomic Ca:Si ratio of the optimum mix is slightly higher than that of the control mix used in this study, the results are very similar to those obtained by [48]. The conversion of calcium hydroxide to additional inclusion of CSH is the primary factor for reducing the Ca:Si ratio of CSH. The optimum mix shows a lower alumina content and similar silica content compared to the control mix. Thus, the optimum mix with recycled aggregate has enhanced strength characteristics. concrete due to its expansion nature during the hydration process. As the hydration time increases up to 28 days, concrete mix densifies substantially. When compared with the control mix, there is no significant difference at 30% replacement of MCRA. An earlier, similar observation was that there was a stronger and denser new interfacial transition zone with fully replaced coarse recycled aggregates and powdered fine recycled aggregate [46]. The interfacial zone ( Figure 7B), which mainly consists of a large densified layer of hydrates, is similar to that observed by [46]. Beyond 30% replacement of MCRA, the amount and distribution of CSH is insufficient. Thus, the increased replacement of the MCRA results in a large amount of porosity and reduced strength of concrete, which can lower the durability properties that can be seen in Mix 3 at 28 days in Figure 7F. CSH gel decalcifies into silica gel, therefore deteriorating the performance of concrete, which can be seen in Figure 7D at 28 days. The increasing amount of silica gel may produce cracks and loss of durability and mechanical strength in concrete structures. In the case of 100% replacement, the SEM images show more nonhydrated particles due to the incomplete reaction caused by the smaller surface area of the mixture, resulting in a less compact microstructure and strength. Therefore, the increased percentage of recycled content results in inferior properties when compared to the natural concrete.  The energy-dispersive X-ray spectroscopy shows the high content of major peaks of Ca, Si, and O, which indicates the presence of calcium silicate hydrates (CSH) in hardened concrete. The high calcium content shown in Figure 8C indicates the presence of a monolithic amorphous CSH similar to the results reported by [47]. The Ca:Si ratio of the optimum and control mix were calculated from the values shown in Figure 8. At 7 days of curing, the Ca:Si ratio is 0.96 and 0.83 for the optimum and control mix, respectively. After a curing time of 28 days, the results indicate that the Ca:Si ratio of the optimum mix is 2.33 when the control mix results in 1.61. Though the atomic Ca:Si ratio of the optimum mix is slightly higher than that of the control mix used in this study, the results are very similar to those obtained by [48]. The conversion of calcium hydroxide to additional inclusion of CSH is the primary factor for reducing the Ca:Si ratio of CSH. The optimum mix shows a lower alumina content and similar silica content compared to the control mix. Thus, the optimum mix with recycled aggregate has enhanced strength characteristics.

X-ray Diffraction
The diffractogram was obtained using CuKα radiation (30 mA and 45 kV), scanning between 10.0100 and 89.1500 (°2Th.), as shown in Table 8. The development of mineral phases formed was assessed after a curing time of 7 and 28 by the XRD technique.

X-ray Diffraction
The diffractogram was obtained using CuKα radiation (30 mA and 45 kV), scanning between 10.0100 and 89.1500 ( • 2Th.), as shown in Table 8. The development of mineral phases formed was assessed after a curing time of 7 and 28 by the XRD technique.

Hydrated Samples at 7 Days
The concrete specimen's X-ray Diffraction (XRD) patterns after seven days of curing are displayed in Figure 9. The control and optimum mix with 30% mixed coarse recycled aggregate have similar patterns. The "X'PERT HIGH SCORE v3.0" software, a commonly used program for the study of the XRD findings, was utilized to analyze the results. This software compares the provided pattern with the reference peaks in the ICDD database and gives the relative intensity of each phase (CSH (C)-PDF Number:33-0306; SiO 2 (Q)-PDF Number: 46-1045; Ca(OH) 2 (P)-PDF Number: 44-1481; CaCO 3 (Ca)-PDF Number: 83-0577), as shown in Table 9. The amount of CSH, CaCO 3 , Ca(OH) 2 [49] with the formation of CSH, CaCO 3 , and Ca(OH) 2 compounds at 29.406 • , 27.233 • , and 34.102 • , respectively. The higher counts of CSH in the optimum mix indicates that the strength improvement is higher than that of the control mix, as shown in Table 9. As reported by [50], as the ettringite is a product of an expansive reaction, additional ettringite formation will hasten the deterioration of recycled aggregate concrete, which is not considerably present in the optimum mixes employed in the current study.

Hydrated Samples at 28 Days
The optimum and control mix's XRD patterns after 28 days of curing are shown in Figure 10. The control and optimum mix have similar patterns. The "X'PERT HIGH SCORE" software compares the provided pattern with the reference peaks in the ICDD database and gives the relative intensity of each phase, as shown in Table 10. While seeing the results obtained from the software and patterns, the phase of Ca(OH) 2 is observed at 18 • and 34 • , which is similar to the observation reported by [51]. It is also observed that the relative peak intensities of portlandite of the optimum mix slightly increase compared with the result obtained for the control specimen. The highest peak of CSH observed in the 2θ value at 27 • is higher than that of the control mix. This result is similar to the results obtained by [52]. The peaks of calcite crystals are found with the highest intensity at 26.60 • for both the control and optimum mix, which is similar to the results observed by [53]. Overall, it is observed that the relative peak intensities of all the crystalline phases in the optimum mix are higher than the peaks obtained in the control specimen, as shown in Table 10.
Number: 83-0577), as shown in Table 9. The amount of CSH, CaCO3, Ca(OH)2, and Al2O3.3H2O are observed at 26.7163°, 28.0422°, 34.1573°, and 18.1007°, respectively, in the optimum mix. Similarly, the amount of CSH, CaCO3, Ca (OH)2, and Al2O3.3H2O are observed at 26.6157°, 27.9707°, 34.0779°, and 18.0160°, respectively, in the control mix. Likewise, similar results were found by [49] with the formation of CSH, CaCO3, and Ca(OH)2 compounds at 29.406°, 27.233°, and 34.102°, respectively. The higher counts of CSH in the optimum mix indicates that the strength improvement is higher than that of the control mix, as shown in Table 9. As reported by [50], as the ettringite is a product of an expansive reaction, additional ettringite formation will hasten the deterioration of recycled aggregate concrete, which is not considerably present in the optimum mixes employed in the current study.

Hydrated Samples at 28 Days
The optimum and control mix's XRD patterns after 28 days of curing are shown in Figure 10. The control and optimum mix have similar patterns. The "X'PERT HIGH SCORE" software compares the provided pattern with the reference peaks in the ICDD database and gives the relative intensity of each phase, as shown in Table 10. While seeing the results obtained from the software and patterns, the phase of Ca(OH)2 is observed at 18° and 34°, which is similar to the observation reported by [51]. It is also observed that the relative peak intensities of portlandite of the optimum mix slightly increase compared with the result obtained for the control specimen. The highest peak of CSH observed in the 2 value at 27° is higher than that of the control mix. This result is similar to the results obtained by [52]. The peaks of calcite crystals are found with the highest intensity at 26.60° for both the control and optimum mix, which is similar to the results observed by [53]. Overall, it is observed that the relative peak intensities of all the crystalline phases in the optimum mix are higher than the peaks obtained in the control specimen, as shown in Table 10.    The peaks of bands in the FTIR spectrum at 7 days were identified based on the observation by [54]. The band of Si-O-Si in the control mix exhibits a stretching vibration at a wavenumber of 962 cm −1 . The replacement of 30% MCRA shifts the Si-O-Si absorption peak toward a higher wavenumber of 978 cm −1 in comparison to the control mix. This shift in wavenumber indicates that the silicon phase in the recycled aggregate changes the Ca:Si ratio in CSH. This could be the reason for the increased compressive strength with the addition of 30% MCRA. The peak at 3643 cm −1 for both mixtures indicates the presence of portlandite (Ca(OH) 2 ), which is revealed by FT-IR spectroscopy. This peak is likely to subside during the period of the exposure, as shown in Figures 11 and 12. The vibration bands at 1684 cm −1 and 3407 cm −1 for the optimum mix indicate that the O-H group is contributed by CSH, but in the control mix, the O-H group is contributed only at 1739 cm −1 . The strong vibration bands at 977 cm −1 and 963 cm −1 for the optimum and control mix, respectively, signify the antisymmetric stretching associated with the Si-O group provided by CSH. The bands at 1379 cm −1 in the control mix and 1400 cm −1 in the optimum mix correspond to the antisymmetric stretching of CO 3 2− . The peak at 1157 and 1206 cm −1 associated with SO 4 2− is detected in the control and optimum mix, respectively, which corresponds to the findings by previous research [55] where the typical sulphate absorption bands were usually present between 1100 and 1200 cm −1 of wavelength because of the v 3 vibration in SO 4 2− . In the current study, there is no sign of AlO 6 at 850 cm −1 , which further reduces the chances of the deterioration of concrete.

Hydrated Samples at 28 Days
The peaks of bands in the FTIR spectrum for both the optimum and control mix at 28 days of hydration are shown in Figure 12. The graph reveals the bond of Si-O located around 817 and 970 cm −1 for the optimum and control mix, respectively, where it was observed between 900 and 1100 cm −1 in the study conducted by previous researchers. Most likely, the small peaks between 600 and 800 cm −1 are brought on by Si-O-Si bonds that come from the original features of the MCRA. It is observed that the intense band at 970 cm −1 is due to the Si-O asymmetric stretching vibration of the CSH. The vibration bands obtained at 1649 cm −1 and 3432 cm −1 for the control mix and 1683 cm −1 and 3436 cm −1 for the optimum mix represent the antisymmetric stretching associated with the OH-group generated by portlandites. The bands of carbonates (CO 3 2− ), CSH, and free silica (O-Si-O) are found to be less than the wavelength of 2000 cm −1 . The presence of the CO 3 2− band at 1365 cm −1 for the control mix and 1372 cm −1 for the optimum mix are found to be approximately similar to each other. The existence of absorption bands between 2960 and 2850 cm −1 that increases the compressive strength of concrete is a sign that stearic acid is present [56]. The considerable C-S-H gel content in both mixes, which is the cause of the strength improvement, is confirmed by FTIR analysis.
addition of 30% MCRA. The peak at 3643 cm −1 for both mixtures indicates the presence of portlandite (Ca(OH)2), which is revealed by FT-IR spectroscopy. This peak is likely to subside during the period of the exposure, as shown in Figures 11 and 12. The vibration bands at 1684 cm −1 and 3407 cm −1 for the optimum mix indicate that the O-H group is contributed by CSH, but in the control mix, the O-H group is contributed only at 1739 cm −1 . The strong vibration bands at 977 cm −1 and 963 cm −1 for the optimum and control mix, respectively, signify the antisymmetric stretching associated with the Si-O group provided by CSH. The bands at 1379 cm −1 in the control mix and 1400 cm −1 in the optimum mix correspond to the antisymmetric stretching of CO3 2-. The peak at 1157 and 1206 cm −1 associated with SO4 2-is detected in the control and optimum mix, respectively, which corresponds to the findings by previous research [55] where the typical sulphate absorption bands were usually present between 1100 and 1200 cm −1 of wavelength because of the v3 vibration in SO4 2-. In the current study, there is no sign of AlO6 at 850 cm −1 , which further reduces the chances of the deterioration of concrete.  The peaks of bands in the FTIR spectrum for both the optimum and control mix at 28 days of hydration are shown in Figure 12. The graph reveals the bond of Si-O located around 817 and 970 cm −1 for the optimum and control mix, respectively, where it was observed between 900 and 1100 cm −1 in the study conducted by previous researchers. Most likely, the small peaks between 600 and 800 cm −1 are brought on by Si-O-Si bonds that come from the original features of the MCRA. It is observed that the intense band at 970 cm −1 is due to the Si-O asymmetric stretching vibration of the CSH. The vibration bands obtained at 1649 cm −1 and 3432 cm −1 for the control mix and 1683 cm −1 and 3436 cm −1 for the optimum mix represent the antisymmetric stretching associated with the OH-group generated by portlandites. The bands of carbonates (CO3 2− ), CSH, and free silica (O-Si-O) are found to be less than the wavelength of 2000 cm −1 . The presence of the CO3 2− band at 1365 cm −1 for the control mix and 1372 cm −1 for the optimum mix are found to be approximately similar to each other. The existence of absorption bands between 2960 and 2850 cm −1 that increases the compressive strength of concrete is a sign that stearic acid is present [56]. The considerable C-S-H gel content in both mixes, which is the cause of the strength improvement, is confirmed by FTIR analysis.

Conclusions
Based on the research findings, the mixed coarse recycled aggregates at 30% replacement can be utilized as an alternative to conventional aggregate to produce recycled aggregate concrete for structural applications. This research can increase the waste utilization in the form of coarse recycled aggregates. Further, the methods for enhancing the mechanical properties can be achieved by the addition of supplementary cementitious

Conclusions
Based on the research findings, the mixed coarse recycled aggregates at 30% replacement can be utilized as an alternative to conventional aggregate to produce recycled aggregate concrete for structural applications. This research can increase the waste utilization in the form of coarse recycled aggregates. Further, the methods for enhancing the mechanical properties can be achieved by the addition of supplementary cementitious materials or various treatment methods, thus contributing to better performance and greater sustainability in construction. This will facilitate the wider use of mixed coarse recycled aggregate in the production of structural concrete as follows.

•
Coarse recycled aggregate satisfied the physical parameters specified in IS 383:2016 for the production of concrete.

•
The incorporation of coarse recycled aggregates in concrete showed a slump value around 75 ± 20 mm.

•
The fresh concrete properties of density with 100% recycled aggregate concrete slightly decreased at a percentage of 2.33%. This behavior was the same for the concrete in fresh and hardened stages.  The mineralogical characterization by X-ray diffraction revealed that the phases found in the recycled aggregates were calcium silicate hydrate, quartz, portlandite, and calcite in the required intensity. • Due to silicate polymerization and the development of calcium silicate hydrate gel, the primary peak at 817 cm −1 changed to a higher frequency 970 cm −1 for the optimum mix as hydration advanced.